6 Progression (vertical) Updeeper penetrationHigher deposit rate (lb/hr)Use near 90 degree travel angle or slightly upDownfaster (point to point)less penetration for thin metalless dilutionUse steep grag angle
7 Travel SpeedStay on the leading edge of the puddle
8 Flat PositionFillet/Groove - stringer or weave, split bead or wide weave
9 HorizontalFillet/Groove - stringers (small weave may be used in tight place)Bead Placement - bottom to top
10 Vertical Fillet/Groove - weave (or whip but not straight stringers) Root pass 6010 whipRoot pass 7018 straight stringer or weave (open closed)
11 Overhead Same as horizontal for Fillets 6010 open root whip for flat face and keyhole control7018’s stringersOH Butt Joints can be stringers or weaves
12 DimensionsReinforcement -ASME flush 1/16 AWS flush 1/8 discuss keyholeing, metallic backing, nonmetallic backing, partial penetration, root openings, root faces, tacking, tack grinding, fast freeze, and fill freezeFill -as many as needed 1/8 per pass flat overload 3/16 verticalCover -flush 1/16 high, 1/16 past edge
13 Butt Joint Preperation (Joints without backing)1/16-1/8600 included angleRoot facesTackingFeather Tacks
14 Open Root TechniqueUse root opening to allow increase in amperage for smoother weldingWhip backwards for penetrationWhip forwards to reduce penetrationDo Not Weave a root pass.Maintain a short arc gapStay slightly in front of the puddle at all times. Use the keyholing technique.
15 Butt Joint Preperation (With Backing)Root faces - 0450 included angleRemove all mill scales and rustTacking - not in grooveTack away from coupon area.Flush on backing
16 Welding grooves with Backing Keep the root opening wideMake the root pass in one beadAvoid tight areas at the weld toes
17 Restarts Stagger all starts and stops or use run-on, run-off tabs Feather all restarts & start on top, or start in front and remeltDon’t restart in a coupon area.Also stagger all beads on a single pass.Use a longer arc length when starting a weld.Compare interpass grinding techniques vs. techniques for no interpass grinding.
18 Craters Fill craters by reversing direction at the weld end Use a short arc length to control heat.
22 Electrode Travel Angles Drag Angle increases PenetrationIncreases crown heightPush Angle gives shallow penetration, and flattens out the weld surface.
23 Electrode (arc) Placement Current takes the path of least resistance. Therefore, the arc, and resulting weld, will go where the electrode end is closest to, NOT NECESSARILY IN THE DIRECTION THE ELECTRODE IS POINTING
24 Arc LengthLonger arc lengths = increased puddle heat, flatter welds, deeper penetrationShorter arc lengths = less puddle heat, flatter welds, less penetrationUse arc length to control puddle size, penetration, and burn through.Normal arc length is 1/16” - 1/8”Use a slightly longer arc length during a start or restart.
25 Helpful Tips Clean your Welding Hood lens Drape the cable over your shoulder or kneeGet ComfortableWatch the puddle, not the arcConcentrate on steady travel speed and arc length
26 SMAW Machine Setup DCEP (also called Direct Current Reverse Polarity) Amp Range#5 fine amperage setting (approximately 110 amps)Connect work leadSet for Constant Current (Variable Voltage)
Your consent to our cookies if you continue to use this website.